Causes, Evaluation, and Repair
of Cracks in Concrete Structures
Reported by ACI Committee 224
American Concrete Institute®
Advancing concrete knowledge
Causes, Evaluation, and Repair of Cracks
in Concrete Structures
Copyright by the American Concrete Institute, Farmington Hills, MI. All rights reserved. This material
may not be reproduced or copied, in whole or part, in any printed, mechanical, electronic, film, or other
distribution and storage media, without the written consent of ACI.
The technical committees responsible for ACI committee reports and standards strive to avoid ambiguities,
omissions, and errors in these documents. In spite of these efforts, the users of ACI documents occa-
sionally find information or requirements that may be subject to more than one interpretation or may be
incomplete or incorrect. Users who have suggestions for the improvement of ACI documents are
requested to contact ACI.
ACI committee documents are intended for the use of individuals who are competent to evaluate the
significance and limitations of its content and recommendations and who will accept responsibility for the
application of the material it contains. Individuals who use this publication in any way assume all risk and
accept total responsibility for the application and use of this information.
All information in this publication is provided “as is” without warranty of any kind, either express or implied,
including but not limited to, the implied warranties of merchantability, fitness for a particular purpose or
ACI and its members disclaim liability for damages of any kind, including any special, indirect, incidental,
or consequential damages, including without limitation, lost revenues or lost profits, which may result
from the use of this publication.
It is the responsibility of the user of this document to establish health and safety practices appropriate to
the specific circumstances involved with its use. ACI does not make any representations with regard to
health and safety issues and the use of this document. The user must determine the applicability of all
regulatory limitations before applying the document and must comply with all applicable laws and regula-
tions, including but not limited to, United States Occupational Safety and Health Administration (OSHA)
health and safety standards.
Order information: ACI documents are available in print, by download, on CD-ROM, through electronic
subscription, or reprint and may be obtained by contacting ACI.
Most ACI standards and committee reports are gathered together in the annually revised ACI Manual of
Concrete Practice (MCP).
American Concrete Institute
38800 Country Club Drive
Farmington Hills, MI 48331
Causes, Evaluation, and Repair of Cracks
in Concrete Structures
Reported by ACI Committee 224
Robert J. Frosch* Jeffrey S. West
Mohamed N. Abou-Zeid Fouad H. Fouad Ralf Leistikow Randall W. Poston
James P. Barlow* Peter A. Lipphardt Royce J. Rhoads
Florian G. Barth David W. Fowler Edward G. Nawy John W. Roberts
J. Floyd Best Grant T. Halvorsen Kamran M. Nemati Andrew Scanlon
David Darwin† Keith A. Pashina Andrea J. Schokker
John F. Duntemann Will Hansen
Harvey H. Haynes*
*Member of task group that prepared these revisions.
†Chair of task group that prepared these revisions.
The causes of cracks in concrete structures are summarized. The proce- Chapter 2—Evaluation of cracking, p. 224.1R-9
dures used to evaluate cracking in concrete and the principal techniques 2.1—Introduction
for the repair of cracks are presented. The key methods of crack repair are 2.2—Determination of location and extent of concrete
discussed, and guidance is provided for their proper application. cracking
2.3—Selection of repair procedures
Keywords: alkali-silica reaction; alkali-carbonate reaction; autogenous
healing; concrete; consolidation; corrosion; cracking (fracturing); drying Chapter 3—Methods of crack repair, p. 224.1R-13
shrinkage; epoxy resins; evaluation; grouting; heat of hydration; mass 3.1—Introduction
concrete; methacrylates; mixture proportion; overlay; plastic; polymer; 3.2—Epoxy injection
precast concrete; prestressed concrete; reinforced concrete; repair; resins; 3.3—Routing and sealing
settlement shrinkage; shrinkage; slab-on-ground; specification; thermal 3.4—Near-surface reinforcing and pinning
expansion; volume change. 3.5—Additional reinforcement
3.6—Drilling and plugging
CONTENTS 3.7—Gravity filling
Preface, p. 224.1R-2 3.8—Grouting
Chapter 1—Causes and control of cracking, 3.10—Crack arrest
p. 224.1R-2 3.11—Polymer impregnation
3.12—Overlay and surface treatments
1.1—Introduction 3.13—Autogenous healing
1.2—Cracking of plastic concrete
1.3—Cracking of hardened concrete Chapter 4—References, p. 224.1R-18
4.1—Referenced standards and reports
ACI Committee Reports, Guides, Standard Practices, and 4.2—Cited references
Commentaries are intended for guidance in planning,
designing, executing, and inspecting construction. This ACI 224.1R-07 supersedes ACI 224.1R-93 and was adopted and published in
document is intended for the use of individuals who are March 2007.
competent to evaluate the significance and limitations of its
content and recommendations and who will accept Copyright © 2007, American Concrete Institute.
responsibility for the application of the material it contains. All rights reserved including rights of reproduction and use in any form or by any
The American Concrete Institute disclaims any and all means, including the making of copies by any photo process, or by electronic or
responsibility for the stated principles. The Institute shall not mechanical device, printed, written, or oral, or recording for sound or visual reproduction
be liable for any loss or damage arising therefrom. or for use in any knowledge or retrieval system or device, unless permission in writing
is obtained from the copyright proprietors.
Reference to this document shall not be made in contract
documents. If items found in this document are desired by the
Architect/Engineer to be a part of the contract documents, they
shall be restated in mandatory language for incorporation by
224.1R-2 ACI COMMITTEE REPORT
PREFACE Fig. 1.1—Typical plastic shrinkage cracking (Price 1982).
Cracks in concrete have many causes. They may affect
appearance only, or they may indicate significant structural Plastic shrinkage cracking is usually associated with the
distress or a lack of durability. Cracks may represent the total rapid loss of moisture caused by a combination of factors
extent of the damage, or they may point to problems of that include high air and concrete temperatures, low relative
greater magnitude. Their significance depends on the type of humidity, and high wind velocity at the surface of the
structure, as well as the nature of the cracking. For example, concrete. Concrete with lower amounts of bleed water, such
cracks that are acceptable for buildings may not be accept- as those containing mineral admixtures (especially silica
able in water-retaining structures. fume) have a greater tendency to undergo plastic shrinkage
Good crack repair techniques depend on knowing the causes cracking than concrete with a greater tendency to bleed.
and selecting appropriate repair procedures that take these
causes into account; otherwise, the repair may only be Because plastic shrinkage cracking is due to a differential
temporary. Successful long-term repair procedures must address volume change in the plastic concrete, successful control
the causes of the cracks as well as the cracks themselves. measures require a reduction in the relative volume change
This report is intended to serve as a tool in the process of between the surface and other portions of the concrete.
crack evaluation and repair of concrete structures.
The causes of cracks in concrete are summarized along Steps can be taken to prevent rapid moisture loss due to
with the principal procedures used for crack control. Both hot weather and dry winds (ACI 224R, 302.1R, and 305R).
plastic and hardened concrete are considered. The impor- These measures include the use of fog nozzles to saturate the
tance of design, detailing, construction procedures, concrete air above the surface and the use of plastic sheeting to cover
proportioning, and material properties are discussed. the surface between finishing operations. Windbreaks to
The techniques and methodology for crack evaluation are reduce the wind velocity and sunshades to reduce the surface
described. The need to determine the causes of cracking as a temperature are also helpful. It is good practice to schedule
necessary prerequisite to repair is emphasized. The selection flatwork after the windbreaks have been erected. During hot,
of successful repair techniques should consider the causes of windy weather with low humidity, it is sometimes advisable
cracking, whether the cracks are active or dormant, and the to reschedule the concrete placement or to initiate concrete
need for repair. Criteria for the selection of crack repair operations at night.
procedures are based on the desired outcome.
Twelve methods of crack repair are presented, including 1.2.2 Settlement cracking—Concrete has a tendency to
the techniques, advantages and disadvantages, and areas of continue to consolidate after initial placement, vibration, and
application for each. finishing. During this period, the plastic concrete may be
locally restrained by reinforcing steel, a previous concrete
CHAPTER 1—CAUSES AND CONTROL placement, or formwork. This local restraint may result in
OF CRACKING voids, cracks, or both, adjacent to the restraining element
(Fig. 1.2). When associated with reinforcing steel, settlement
1.1—Introduction cracking increases with increasing bar size, increasing
This chapter presents a brief summary of the causes of slump, and decreasing cover (Dakhil et al. 1975); this is
shown in Fig. 1.3 for a limited range of these variables. The
cracks and means for their control. Cracks are categorized as degree of settlement cracking may be intensified by insufficient
occurring either in plastic concrete or hardened concrete vibration or by the use of leaking or highly flexible forms.
(Kelly 1981; Price 1982). In addition to the information Suprenant and Malisch (1999) demonstrated that the addition
provided herein, further details are presented in ACI 224R of fibers can reduce the formation of settlement cracks.
and articles by Carlson et al. (1979), Kelly (1981), Price
(1982), and Abdun-Nur (1983). Additional references are The following items will reduce settlement cracking:
cited throughout the chapter. • Form design following ACI 347;
• Concrete vibration (and revibration) (ACI 309R);
1.2—Cracking of plastic concrete • Provision of a time interval between the placement of
1.2.1 Plastic shrinkage cracking—When moisture evapo-
concrete in columns or deep beams and the placement
rates from the surface of freshly placed concrete faster than of concrete in slabs and beams (ACI 309.2R);
it is replaced by bleed water, the surface concrete shrinks.
Due to the restraint provided by the concrete below the
drying surface layer, tensile stresses develop in the weak,
stiffening plastic concrete. This results in shallow cracks of
varying depths that may form a random, polygonal pattern,
or be essentially parallel to one another (Fig. 1.1). These
cracks may be fairly wide (as much as 1/8 in. [3 mm]) at the
surface. They range from a few inches to many feet in length,
and are spaced from a few inches (millimeters) to as much as
10 ft (3 m) apart. Plastic shrinkage cracks begin as shallow
cracks, but can become full-depth cracks later in the life of
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-3
• Use of the lowest possible slump;
• An increase in concrete cover; and
• Addition of fibers.
1.3—Cracking of hardened concrete Fig. 1.2—Crack formed due to obstructed settlement
1.3.1 Drying shrinkage—A common cause of cracking in (Price 1982).
concrete is restrained drying shrinkage. Drying shrinkage is Fig. 1.3—Settlement cracking as a function of bar size,
caused by the loss of moisture from the cement paste constit- slump, and cover (Dakhil et al. 1975).
uent, which can shrink by as much as 1%. Fortunately, cracking may also be reduced or even eliminated by using
aggregate particles provide internal restraint that reduces the shrinkage-compensating cement or a shrinkage-compensating
magnitude of this volume change to about 0.06%. On the admixture. The reduction or elimination of subslab restraint
other hand, concrete tends to expand when wetted (the can also be effective in reducing shrinkage cracking in slabs-
volume increase can be the same order of magnitude as that on-ground (Wimsatt et al. 1987). In cases where crack
observed due to shrinkage). control is particularly important, the minimum requirements
of ACI 318 may not be adequate. These points are discussed
These moisture-induced volume changes are a characteristic in greater detail in ACI 224R, which describes additional
of concrete. If the shrinkage of concrete could take place construction practices designed to help control the drying
without restraint, the concrete would not crack. It is the shrinkage cracking that does occur, and in ACI 224.3R,
combination of shrinkage and restraint (provided by another which describes the use and function of joints in concrete
part of the structure, by the subgrade, or by the moist interior construction.
of the concrete itself) that causes tensile stresses to develop.
When the tensile strength of the material is exceeded, concrete Autogenous shrinkage “is a special case of drying
will crack. Cracks may propagate at much lower stresses than shrinkage” (Mindess et al. 2003) that results from self-desic-
are required to cause crack initiation (ACI 446.1R). cation (internal drying) in concretes with water-cementitious
material ratios (w/cm) below 0.42, but most often observed
In massive concrete elements, tensile stresses are caused by at a w/cm below 0.30. Thus, it is a problem often associated
differential shrinkage between the surface and the interior with high-strength concretes. Autogenous shrinkage occurs
concrete. The higher shrinkage at the surface causes cracks to without the loss of moisture from the bulk concrete.
develop that may, with time, penetrate deeper into the concrete.
The magnitude of the tensile stresses induced by volume
change is influenced by a combination of factors, including
the amount and rate of shrinkage, the degree of restraint, the
modulus of elasticity, and the amount of creep. The amount
of drying shrinkage is influenced mainly by the amount and
type of aggregate and the cement paste (cement and water)
content of the mixture. As the quantity of aggregate
increases, the shrinkage decreases (Pickett 1956). The higher
the stiffness of the aggregate, the more effective it is in
reducing the shrinkage of the concrete; that is, the shrinkage
of concrete containing sandstone aggregate may be more
than twice that of concrete with granite, basalt, or high-
quality limestone (Carlson 1938). The higher the water and
cement contents, the greater the amount of drying shrinkage
(U.S. Bureau of Reclamation 1975; Schmitt and Darwin
1999; Darwin et al. 2004).
Surface crazing (alligator pattern) on walls and slabs is an
example of drying shrinkage on a small scale. Crazing
usually occurs when the surface layer of the concrete has a
higher water content than the interior concrete. The result is
a series of shallow, closely spaced, fine cracks.
A procedure that will help reduce settlement cracking, as
well as drying shrinkage in walls, is reducing the water
content of the concrete as the wall is placed from the bottom
to the top (U.S. Bureau of Reclamation 1975; ACI 304R).
Using this procedure, bleed water from the lower portions of
the wall will tend to equalize the water content within the
wall. To be successful, this procedure needs careful control
of the concrete and proper consolidation.
Shrinkage cracking can be controlled by using contraction
joints and proper detailing of the reinforcement. Shrinkage
224.1R-4 ACI COMMITTEE REPORT
The self-desiccation occurs as the relative humidity in 2001; ACI 343R). Allowing for movement by using properly
interior voids drops to 75 to 80%, which results in bulk designed contraction and isolation joints and correct
shrinkage. Autogenous shrinkage strain is typically about 40 detailing will help alleviate these problems.
to 100 × 10–6 (Davis 1940), but has been measured as high
as 2300 × 10–6 for concrete with a w/cm of 0.20 (Ai 2000). 1.3.3 Chemical reaction—Deleterious chemical reactions
Houk et al. (1969) found that autogenous shrinkage may cause cracking of concrete. These reactions may be due
increases with increasing temperature, cement content, and to materials used to make the concrete or materials that come
cement fineness. into contact with the concrete after it has hardened.
1.3.2 Thermal stresses—Temperature differences within a Some general concepts for reducing adverse chemical
concrete structure may be caused by portions of the structure reactions are presented herein, but only pretesting of the
losing heat of hydration at different rates or by the weather mixture or extended field experience will determine the
conditions cooling or heating one portion of the structure to effectiveness of a specific measure.
a different degree or at a different rate than another portion
of the structure. These temperature differences result in Concrete may crack with time as the result of slowly
differential volume changes. When the tensile stresses due to developing expansive reactions between aggregate
the differential volume changes exceed the tensile strength, containing active silica and alkalis derived from cement
concrete will crack. Temperature differentials and the hydration, admixtures, or external sources (such as curing
accompanying volume changes due to the dissipation of the water, groundwater, deicing chemicals, and alkaline solutions
heat of hydration of cement are normally associated with stored or used in the finished structure).
mass concrete (which can include large columns, piers,
beams, and footings, as well as dams), whereas temperature When the alkalis in cement react with susceptible aggregate
differentials due to changes in the ambient temperature can particles, a reaction rim of alkali-silica gel is formed around
affect any structure. the aggregate. If this gel is exposed to moisture, it expands,
causing an increase in volume of the concrete mass that will
Cracking in mass concrete can result from a greater result in cracking and may eventually result in the complete
temperature on the interior than on the exterior. The temper- deterioration of the structure. Control measures include
ature gradient may be caused by either the center of the using nonreactive aggregates, low-alkali cement, and
concrete heating more than the outside due to the liberation pozzolans that consist principally of very fine, highly active
of heat during cement hydration or more rapid cooling of the silica. The first measure may preclude the problem from
exterior relative to the interior. Both cases result in tensile occurring, while the later two measures have the effect of
stresses on the exterior and, if the tensile strength is decreasing the alkali-reactive silica ratio, resulting in the
exceeded, cracking will occur. The tensile stresses are formation of a nonexpanding calcium alkali silicate hydrate.
proportional to the temperature differential, the coefficient
of thermal expansion, the effective modulus of elasticity Certain carbonate rocks participate in reactions with
(which is reduced by creep), and the degree of restraint alkalis that, in some instances, produce detrimental expansion
(Dusinberre 1945; Houghton 1972, 1976). The more and cracking. These detrimental alkali-carbonate reactions
massive the structure, the greater the potential for temperature are usually associated with argillaceous dolomitic limestones
differential and restraint. that have a very fine-grained (cryptocrystalline) structure
(ACI 201.2R). The affected concrete is characterized by a
Procedures to help reduce thermally induced cracking network pattern of cracks. The reaction is distinguished from
include reducing the maximum internal temperature, the alkali-silica reaction by the general absence of silica gel
delaying the onset of cooling, controlling the rate at which surface deposits at the crack. The problem may be minimized
the concrete cools, and increasing the tensile strength of the by avoiding reactive aggregates, dilution with nonreactive
concrete. These and other methods used to reduce cracking aggregates, use of a smaller maximum size aggregate, and
in massive concrete are presented in ACI 207.1R, 207.2R, use of low-alkali cement (ACI 201.2R).
207.4R, and 224R.
Sulfates in soil and water are a special durability problem
Hardened concrete has a coefficient of thermal expansion for concrete. When sulfate penetrates hydrated cement paste,
that may range from 3 to 7 × 10–6/°F (6 to 13 × 10–6/°C), it comes in contact with hydrated calcium aluminate.
with a typical value of 5.5 × 10–6/°F (10 × 10–6/°C). When Calcium sulfoaluminate is formed, which may result in an
one portion of a structure is subjected to a temperature- increase in volume. The resulting expansion may cause the
induced volume change, the potential for thermally induced development of closely spaced cracks and the eventual
cracking exists. Designers should give special consideration deterioration of the concrete. ASTM C 150 Types II and V
to structures in which some portions are exposed to temper- portland cement, which are low in tricalcium aluminate, will
ature changes, while other portions of the structure are either minimize the formation of calcium sulfoaluminate. Sulfate-
partially or completely protected. A drop in temperature may resistant cements specified in ASTM C 595 and C 1157 are
result in cracking in the exposed element, whereas increases also useful in improving sulfate resistance. Pozzolans that
in temperature may cause cracking in the protected portion have been tested and shown to impart additional resistance to
of the structure. Temperature gradients cause deflection and sulfate attack are beneficial. Using concrete with a low w/cm is
rotation in structural members; if restrained, serious stresses important to providing protection against severe sulfate attack.
can result (Priestley 1978; Hoffman et al. 1983; Haynes
Detrimental conditions may also occur from the application
of deicing salts to the surface of hardened concrete. Chlorides
from deicing chemicals can permeate concrete, reducing the
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-5
ability of the concrete protect embedded reinforcement from Reinforcing steel usually does not corrode in concrete because
corrosion. Because corrosion products occupy a greater a tightly adhering protective oxide coating forms in the highly
volume than the original metal, corrosion can lead to delam- alkaline environment. This is known as passive protection.
ination and cracking of the concrete. Deicing salts also make
concrete more susceptible to freezing-and-thawing damage. Reinforcing steel may corrode, however, if the alkalinity
To limit these effects, concrete subjected to water-soluble of the concrete is reduced through carbonation or if the
salts should be amply air entrained, have adequate cover of passivity of this steel is destroyed by aggressive ions
the reinforcing steel, and be made of high-quality, low- (usually chlorides). Corrosion of the steel produces iron
permeability concrete. oxides and hydroxides that have a volume much greater than
the volume of the original metallic iron (Bentur et al. 1997).
The effects of these and other problems relating to the This increase in volume causes high radial bursting stresses
durability of concrete are discussed in greater detail in around reinforcing bars and results in local radial cracks.
ACI 201.2R. These splitting cracks can propagate along the bar, resulting in
the formation of longitudinal cracks (parallel to the bar) or
The calcium silicate hydrate and calcium hydroxide in spalling of the concrete. A broad crack may also form at a
hydrated cement paste will combine with carbon dioxide in plane of bars parallel to a concrete surface, resulting in delam-
the air to form calcium carbonate. When this occurs, the ination, which is a well-known problem in bridge decks.
concrete undergoes irreversible carbonation shrinkage,
which may result in surface crazing. In addition, freshly Cracks provide easy access for oxygen, moisture, and
placed concrete surfaces exposed (during the first 24 hours) chlorides; thus, minor splitting (longitudinal) cracks can
to carbon dioxide from improperly vented combustion create a condition in which corrosion and cracking are
heaters, used to keep concrete warm during the winter accelerated. Cracks transverse to reinforcement do not
months, are susceptible to dusting. usually cause continuing corrosion of the reinforcement if
the concrete has low permeability. The exposed portion of a
1.3.4 Weathering—The weathering processes that can bar at a crack acts as an anode. At early ages, local corrosion
cause cracking include freezing and thawing, wetting and occurs; the wider the crack, the greater the corrosion,
drying, and heating and cooling. Damage from freezing and because a greater portion of the bar has lost its passive
thawing is the most common weather-related physical protection. For continued corrosion to occur, however,
deterioration. Concrete may be damaged by freezing of oxygen and moisture must be supplied to other portions of
water in the paste, in the aggregate, or in both (Powers 1975). the same bar or bars that are electrically connected by direct
contact or through hardware, such as chair supports. If the
Damage in hardened cement paste from freezing is caused combination of density and cover thickness is adequate to
by the movement of water to freezing sites and, for water in restrict the flow of oxygen and moisture, then the corrosion
larger voids, by hydraulic pressure generated by the growth process is self-sealing (Verbeck 1975).
of ice crystals (Powers 1975).
Corrosion can continue if a longitudinal crack forms
Aggregate particles are surrounded by cement paste, parallel to the reinforcement because passivity is lost at
which prevents the rapid escape of water. When the aggregate many locations and oxygen and moisture are readily
particles are above a critical degree of saturation, the available along the full length of the crack.
expansion of the absorbed water during freezing may crack
the surrounding cement paste or damage the aggregate itself Other causes of longitudinal cracking, such as high bond
(Callan 1952; Snowdon and Edwards 1962). stresses, transverse tension (for example, along stirrups or
along slabs with two-way tension), shrinkage, and settlement,
Concrete is best protected against freezing and thawing can initiate corrosion.
through the use of the lowest practical w/cm and total water
content, durable aggregate, and adequate air entrainment. For general concrete construction, the best protection
Adequate curing before exposure to freezing conditions is against corrosion-induced splitting is the use of concrete
also important. Allowing the structure to dry after curing will with low permeability and adequate cover. Increased
enhance its freezing-and-thawing durability. concrete cover over the reinforcement is effective in
delaying the corrosion process by limiting carbonation, as
Other weathering processes that may cause cracking in well as access by oxygen, moisture, and chlorides, and also
concrete are alternate wetting and drying, and heating and in resisting the splitting and spalling caused by corrosion or
cooling. Both processes produce volume changes that may transverse tension (Gergely 1981; Beeby 1983). In the case
cause cracking. If the volume changes are excessive, cracks of large bars and thick covers, it may be necessary to add
may occur, as discussed in Sections 1.3.1 and 1.3.2. small transverse reinforcement (while maintaining the
minimum cover requirements) to limit splitting and to reduce
1.3.5 Corrosion of reinforcement—Corrosion of a metal is the surface crack width (ACI 345R).
an electrochemical process that requires an oxidizing agent,
moisture, and electron flow within the metal; a series of In very severe exposure conditions, additional protective
chemical reactions takes place on and adjacent to the surface measures may be required. A number of options are available,
of the metal (ACI 201.2R and 222R). such as coated reinforcement, sealers, or overlays on the
concrete, corrosion-inhibiting admixtures, and cathodic
The key to protecting metal from corrosion is to stop or protection (Transportation Research Board 1979). Any
reverse the chemical reactions. This may be done by cutting procedure that effectively prevents access of oxygen and
off the supplies of oxygen or moisture or by supplying
excess electrons at the anodes to prevent the formation of the
metal ions (cathodic protection).
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-7
detensioned immediately after the steam curing has been Fig. 1.4—Typical crack patterns at re-entrant corners
discontinued (PCI Energy Committee 1981). (Price 1982).
Cast-in-place concrete can be unknowingly subjected to Fig. 1.5—Typical cracking pattern of dapped end beam at
construction loads in cold climates when heaters are used to service load (Mattock and Chan 1979).
provide an elevated working temperature within a structure.
Typically, tarps are used to cover windows and door openings, The restraint of members subjected to volume changes
and high-volume heaters are operated inside the enclosed frequently results in cracks. Stresses that can occur in
area. If the heaters are located near exterior concrete members, concrete due to restrained creep, temperature differential,
especially thin walls, an unacceptably high thermal gradient and drying shrinkage can be many times the stresses that
can result within the members. The interior of the wall will occur due to loading. A slab, wall, or a beam restrained
expand in relation to the exterior. Heaters should be kept away against shortening, even if prestressed, can easily develop
from the exterior walls to minimize this effect. Good practice tensile stresses sufficient to cause cracking. Properly
also requires that this be done to avoid localized drying designed walls should have contraction joints spaced from
shrinkage and carbonation cracking. one to three times the wall height. Beams should be allowed
to move. Cast-in-place post-tensioned construction that does
Storage of materials and the operation of equipment can not permit shortening of the prestressed member is susceptible
easily result in loading conditions during construction far to cracking in both the member and the supporting structure
more severe than any load for which the structure was (Libby 1977). The problem with restraint of structural members
designed. Tight control should be maintained to avoid is especially serious in pretensioned and precast members that
overloading conditions. Damage from unintentional may be welded to the supports at both ends. When combined
construction overloads can be prevented only if designers with other problem details (such as re-entrant corners), results
provide information on load limitations for the structure and if may be catastrophic (Kaminetzky 1981; Mast 1981).
construction personnel heed these limitations.
Improper foundation design may result in excessive differ-
1.3.8 Errors in design and detailing—The effects of ential movement within a structure. If the differential
improper design or detailing range from poor appearance to
lack of serviceability to catastrophic failure. These problems
can be minimized only by a thorough understanding of struc-
tural behavior (meant herein in the broadest sense).
Errors in design and detailing that may result in unacceptable
cracking include use of poorly detailed re-entrant corners in
walls, precast members, and slabs; improper selection or
detailing of reinforcement, or both; restraint of members
subjected to volume changes caused by variations in temper-
ature and moisture; lack of adequate contraction joints; and
improper design of foundations, resulting in differential
movement within the structure. Examples of these problems
are presented by Kaminetzky (1981) and Price (1982).
Re-entrant corners provide a location for the concentration
of stress and, therefore, are prime locations for the initiation
of cracks. Whether the high stresses result from volume
changes, in-plane loads, or bending, the designer should
recognize that stresses are always high near re-entrant
corners. Well-known examples are window and door openings
in concrete walls and dapped-end beams, as shown in Fig. 1.4
and 1.5. Additional properly anchored diagonal reinforcement
is required to keep the inevitable cracks narrow and prevent
them from propagating.
The use of an inadequate amount of reinforcement may
result in excessive cracking. A typical mistake is to lightly
reinforce a member because it is a nonstructural member.
The member (such as a wall), however, may be tied to the
rest of the structure in such a manner that it is required to
carry a major portion of the load once the structure begins to
deform. The nonstructural element then begins to carry loads
in proportion to its stiffness. Because this member is not
detailed to act structurally, unsightly cracking may result
even though the safety of the structure is not in question. In
some cases, it may be advisable to isolate a nonstructural
element from the structural system.
224.1R-8 ACI COMMITTEE REPORT
movement is relatively small, the cracking problems may be corrosion of reinforcement; however, these limits do not
only visual in nature. If there is a major differential settle- appear to be justified on the basis of corrosion control.
ment, however, the structure may not be able to redistribute
the loads rapidly enough, and a failure may occur. One of the A re-evaluation of cracking data provided a new crack
advantages of reinforced concrete is that if the movement width equation based on a physical model (Frosch 1999). For
takes place over a long enough period of time, creep will the calculation of maximum crack widths, the crack width
allow at least some load redistribution to take place. can be calculated as
The importance of proper design and detailing will depend w = 2-f--s- β dc2 ⎛ -2s-⎞⎠ 2
on the particular structure and loading involved. Special care Es ⎝
should be taken in the design and detailing of structures in + (1-2)
which cracking may cause a major serviceability problem.
These structures also require continuous inspection during where
all phases of construction to supplement the careful design
and detailing. w = maximum crack width, in. (mm);
1.3.9 Externally applied loads—It is well known that load- fs = reinforcing steel stress, ksi (MPa);
induced tensile stresses result in cracks in concrete members. Es = reinforcing steel modulus of elasticity, ksi (MPa);
This point is readily acknowledged and accepted in the β = ratio of distance between neutral and tension face to
design of reinforced concrete structures. Current design
procedures (ACI 318 and the AASHTO “Standard Specifi- distance between neutral axis and centroid of rein-
cation for Highway Bridges”) use reinforcing steel not only forcing steel (taken as approximately 1.0 + 0.08dc);
to carry the tensile forces, but to obtain both an adequate dc = thickness of cover from tension face to center of
distribution of cracks and a reasonable limit on crack width. closest bar, in. (mm); and
Experimental evidence provides the basis for the s = bar spacing, in. (mm).
following general conclusions about the variables that
control cracking in flexural members: crack width increases Crack control is achieved in ACI 318 through the use of a
with increasing steel stress, cover thickness, and area of spacing criterion for reinforcing steel that is based on the
concrete surrounding each reinforcing bar. Of these, steel stress under service conditions and clear cover on the bars.
stress is the most important variable. The bar diameter is not This design equation was based on Eq. (1-2), considering
a major consideration. The width of a bottom crack increases crack widths on the order of 0.016 in. (0.40 mm).
with an increasing strain gradient between the steel and the
tension face of the beam. ACI 318 also includes provisions to prevent the formation
of cracks in regions away from the location of the main
The equation that is often used to predict the most probable reinforcement through the provision of skin reinforcement in
maximum surface crack width in bending was developed by the webs of beams that are deeper than 36 in. (900 mm) and
Gergely and Lutz (1968). A simplified version of this equation is the distribution of negative moment reinforcement within
the effective width of a flange in tension. ACI 318 also
w = 0.076βfs 3 dcA × 10–3 (in.-lb) (1-1) requires that, in cases where the primary flexural reinforcement
in a slab that is acting as a T-beam flange is parallel to the
w = 0.046βfs 3 dcA × 10–6 (SI) beam, reinforcement perpendicular to the beam should be
provided in the top of the slab. The transverse reinforcement
where in the slab is designed to carry the factored load on an
w = most probable maximum crack width, in. (mm); overhanging slab width that is assumed to act as a cantilever.
β = ratio of distance between neutral axis and tension For isolated beams, the full width of the overhang is
considered. For other T-beams, the effective width of the
face to distance between neutral axis and centroid of flange is used to design the transverse reinforcement.
reinforcing steel (taken as approximately 1.20 for
typical beams in buildings); There have been a number of crack width equations
fs = reinforcing steel stress, ksi (MPa); developed for prestressed concrete members (ACI 224R),
dc = thickness of cover from tension fiber to center of the but no single method has achieved general acceptance.
closest bar, in. (mm); and
A = area of concrete symmetric with reinforcing steel The maximum crack width in tension members is larger
divided by number of bars, in.2 (mm2). than that predicted by the expression for flexural members
A modification of this equation is used in the AASHTO (Broms 1965; Broms and Lutz 1965). Absence of a strain
bridge specification, which effectively limits crack widths to gradient and compression zone in tension members is the
0.015 or 0.012 in. (0.38 or 0.30 mm), depending on the probable reason for the larger crack widths.
exposure condition. Considering the information presented
in Section 1.3.5 that indicates little correlation between On the basis of limited data, the following expression has
surface crack width for cracks transverse to bars and the been suggested to estimate the maximum crack width in
direct tension (ACI 224R).
w = 0.10fs 3 dcA × 10–3 (in.-lb) (1-3)
w = 0.0605fs 3 dcA × 10–3 (SI)
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-9
Additional information on cracking of concrete in direct Fig. 2.1—Comparator for measuring crack widths (courtesy
tension is provided in ACI 224.2R. of Edmound Scientific Co.).
Flexural and tensile crack widths can be expected to increase
with time for members subjected to either sustained or repetitive
loading. Although a large degree of scatter is evident in the avail-
able data, a doubling of crack width with time can be expected
(Abeles et al. 1968; Bennett and Dave 1969; Illston and Stevens
1972; Holmberg 1973; Rehm and Eligehausen 1977).
The basic principles of crack control for load-induced
cracks are well understood. Well-distributed reinforcement
offers the best protection against undesirable cracking.
Reduced steel stress, obtained through the use of a larger
amount of steel, will reduce crack width. While reduced
cover will reduce the surface crack width, designers should
keep in mind, as pointed out in Section 1.3.5, that cracks (and
therefore, crack widths) perpendicular to reinforcing steel do
not have a major effect on the corrosion of the steel, while a
reduction in cover will be detrimental to the corrosion
protection of the reinforcement.
CHAPTER 2—EVALUATION OF CRACKING Fig. 2.2—Card used to measure crack width (courtesy of
2.1—Introduction Construction Technology Laboratories).
When anticipating repair of cracks in concrete, it is important A grid marked on the surface of the structure can be useful
to first identify the location and extent of cracking. It should to accurately locate cracks on the sketch.
be determined whether the cracks are indicative of current or
future structural problems, taking into consideration both Crack widths can be measured to an accuracy of approx-
present and anticipated loading conditions. The cause of the imately 0.001 in. (0.025 mm) using a crack comparator,
cracking should be established before repairs are specified. which is a small, hand-held microscope with a scale on the
Drawings, specifications, and construction and maintenance lens closest to the surface being viewed (Fig. 2.1). It is gener-
records should be reviewed. If these documents, along with ally more convenient, however, to estimate crack widths
field observations, do not provide the needed information, a using a clear card having lines of specified width marked on
field investigation and structural analysis should be the card, as shown in Fig. 2.2. Any displacement of the
completed before proceeding with repairs. surface (change in elevation) across the crack should also be
documented. Observations such as spalling, exposed rein-
The causes of cracks are discussed in Chapter 1. A detailed forcement, surface deterioration, and rust staining should be
evaluation of observed cracking can determine which of the noted on the sketch. Internal conditions at specific crack
causes applies in a particular situation. locations can be observed with the use of flexible shaft fiber-
scopes or rigid borescopes.
Cracks need to be repaired if they reduce the strength,
stiffness, or durability of the structure to an unacceptable Crack movement can be monitored with mechanical
level, or if the function of the structure is seriously impaired. movement indicators of the types shown in Fig. 2.3. The
In some cases, such as cracking in water-retaining structures, indicator, or crack monitor, shown in Fig. 2.3(a) gives a
the function of the structure will dictate the need for repair, direct reading of crack displacement and rotation. The indi-
even if strength, stiffness, and appearance are not seriously cator in Fig. 2.3(b) (Stratton et al. 1978) amplifies the crack
impaired. Cracks in pavements and slabs-on-ground may
require repair to prevent edge spalls or the migration of water
to the subgrade, or to maintain intended load-carrying
capacity. In addition, repairs that improve the appearance of
the surface of a concrete structure may be desired.
2.2—Determination of location and extent
of concrete cracking
Location and extent of cracking as well as information on the
general condition of concrete in a structure can be determined
by both direct and indirect observations, nondestructive
testing, and destructive tests such as test cores taken from the
structure. Information may also be obtained from drawings
and construction and maintenance records.
2.2.1 Direct and indirect observation—The locations and
widths of cracks should be noted on a sketch of the structure.
224.1R-10 ACI COMMITTEE REPORT
Fig. 2.3—(a) Crack monitor (courtesy of Avongard); and (b) crack movement indicator
(Stratton et al. 1978).
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-11
movement (in this case, 50 times) and indicates the Fig. 2.4—Pachometer (reinforcing bar indicator) (courtesy
maximum range of movement during the measurement of James Instruments).
period. Mechanical indicators have the advantage that they
do not require moisture protection. If more detailed time When access is not available to opposite faces, transducers
histories are desired, a wide range of transducers (most may be located on the same face (Fig. 2.5(a)). While this
notably, linear variable differential transformers [LVDTs]) technique is possible, the interpretation of results is not
and data-acquisition systems (ranging from strip chart straightforward.
recorders to computer-based systems) are available.
A significant change in measured pulse velocity can occur
Sketches can be supplemented by photographs documenting if an internal discontinuity results in an increase in path
the condition of the structure at the time of investigation. length for the signal. Generally, the higher the pulse velocity,
Guidance for making a condition survey of concrete in the higher the quality of the concrete. The interpretation of
service is given in ACI 201.1R, 201.3R, 207.3R, 345.1R, pulse velocity test results is significantly improved with the
and 546.1R. use of an oscilloscope that provides a visual representation
of the received signal (Fig. 2.5(b)).
2.2.2 Nondestructive testing—Nondestructive tests can be
made to determine the presence of internal cracks and voids Some equipment provides only a digital readout of the
and the depth of penetration of cracks visible at the surface. pulse travel time with no oscilloscope display. If no signal
arrives at the receiving transducer, a significant internal
Tapping the surface with a hammer or using a chain drag discontinuity, such as a crack or void, is indicated. An indi-
are simple techniques to identify laminar cracking near the cation of the extent of the discontinuity can be obtained by
surface. A hollow sound indicates one or more cracks below taking readings at a series of positions on the member.
and parallel to the surface. Infrared imaging equipment,
though expensive, has also proven to be useful in identifying Ultrasonic equipment should be operated by trained
regions in which concrete has delaminated. personnel, and the results should be evaluated cautiously by
an experienced individual because moisture, reinforcing
The presence of reinforcement can be determined using a steel, and embedded items may affect the results. For example,
pachometer (Fig. 2.4). A number of pachometers are available with fully saturated cracks, ultrasonic testing will generally be
that range in capability from merely indicating the presence ineffective, and in some cases, it is difficult to discern between
of steel to those that may be calibrated to allow the experienced a group of narrow cracks and a single large crack.
user a closer determination of depth and the size of reinforcing
steel. In some cases, however, it may be necessary to remove An alternative to through-transmission testing is the pulse-
the concrete cover (often by drilling or chipping) to identify echo technique in which a simple transducer is used to send
the bar sizes or to calibrate cover measurements, especially and receive ultrasonic waves. It has, however, been difficult
in areas of congested reinforcement. Newer devices use to develop a practical pulse-echo test for concrete. Pitch-
magnetic fields and computer algorithms to provide a visual catch systems have been developed that use separate trans-
picture of the reinforcing bar layout in the scanned area. This mitting and receiving transducers (Alexander 1980). More
device can be used to detect reinforcement, measure
concrete cover, and determine the reinforcement size and
position (ACI 228.2R).
If corrosion is a suspected cause of cracking, the easiest
approach to investigate for corrosion entails the removal of a
portion of the concrete to directly observe the steel. Corrosion
potential can be detected by electrical potential measurements
using a suitable reference half-cell. The most commonly
used is a copper-copper sulfate half-cell (ASTM C 876); its
use also requires access to a portion of the reinforcing steel.
The half-cell technique, however, is sensitive to the moisture
condition of the concrete, and if readings are taken when the
concrete is dry, half-cell potentials may indicate no corrosion
activity when, in fact, the steel is undergoing corrosion.
With properly trained personnel and careful evaluation, it
is possible to detect cracks using ultrasonic nondestructive
test equipment (ASTM C 597). The most common technique
is through-transmission testing using commercially available
equipment (Malhotra and Carino 2004; Knab et al. 1983). A
mechanical pulse is transmitted to one face of the concrete
member and received at the opposite face, as shown in
Fig. 2.5. The time taken for the pulse to pass through the
member is measured electronically. If the distance between
the transmitting and receiving transducers is known, the
pulse velocity can be calculated.
224.1R-12 ACI COMMITTEE REPORT
Fig. 2.5—Ultrasonic testing: through-transmission technique. Fig. 2.6—Impact-echo response of a solid plate: (a) schematic
of test configuration; (b) displacement waveform; (c) ampli-
detailed information on pulse-echo and other wave propagation tude spectrum; and (d) normalized amplitude spectrum.
methods is provided by Malhotra and Carino (2004).
to the radiation. Gamma-ray equipment is less expensive and
Significant advances in use of wave propagation techniques relatively portable compared with x-ray equipment and,
for flaw detection in concrete by the impact-echo technique therefore, appears to be more suitable for field testing.
have been made (Sansalone and Carino 1988, 1989;
Sansalone 1997). A mechanical pulse is generated by impact Ground-penetrating radar (GPR), also called impulse
on one face of the member, as illustrated in Fig. 2.6. The radar, uses electromagnetic waves to measure discontinuities
wave propagates through the member, reflects from a defect below a concrete surface. The technique has been used to
or other surface of the member, and is received by a locate cracks, voids, reinforcing steel, and to measure thick-
displacement transducer placed near the impact point. ness. “Due to the large number of physical properties
Figure 2.6(b) shows a surface time-domain waveform affecting the received signal,” however, “current application
received by the transducer. A resonance condition is set up to structural concrete (other than measurements of the spatial
in the member between the member boundaries or boundary configuration of concrete and reinforcement) is largely
and defect. By analyzing the frequency content of the time- restricted to qualitative comparative uses” (ACI 228.2R).
domain waveform (Fig. 2.6(c)), the frequency associated with
the resonance appears as a peak amplitude. In the case of An important use of nondestructive testing is finding those
Fig. 2.6(a), the peak is that associated with the thickness portions of the structure that require a more detailed investi-
frequency (Fig. 2.6(d)). If an internal flaw exists, then a gation, which may include core tests.
significant amplitude peak from the reflections from the flaw
depth will be observed at the associated flaw depth frequency. 2.2.3 Tests on concrete cores—Significant information
can be obtained from cores taken from selected locations
Radiography can also be used to detect internal disconti- within the structure. Cores and core holes afford the oppor-
nuities. Both x-ray and gamma-ray equipment is available tunity to accurately measure the width and depth of cracks.
(Malhotra and Carino 2004; Bungey 1990). The procedures In addition, an indication of concrete quality can be obtained
are best suited for detecting crack planes parallel to the direction from compressive strength tests; however, cores that contain
of radiation; it is difficult to discern crack planes perpendicular cracks should not be used to determine concrete strength.
Petrographic examinations (ASTM C 856) of cracked
concrete can identify material causes of cracking, such as
alkali reactivity, cyclic freezing damage, D-cracking, expansive
aggregate particles, fire-related damage, shrinkage, and
corrosion. Petrography can also identify other factors that
may be related to cracking, such as the w/cm, relative paste
volume, and distribution of concrete components. Petrography
can frequently determine the relative age of cracks and can
identify secondary deposits on fracture surfaces, which have
an influence on repair schemes.
Chemical tests for the presence of excessive chlorides indi-
cate the potential for corrosion of embedded reinforcement.
2.2.4 Review of drawings and construction data—The
original structural design, reinforcement placing, and other
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-13
construction drawings should be reviewed to confirm that the settlement, repair will be of no use until the settlement
concrete thickness and quality, along with the reinforcement, problem is corrected.
meets or exceeds strength and serviceability requirements
noted in the governing building code(s). The actual loading This chapter provides a survey of crack repair methods,
should be compared with design loads. Concrete configurations, including a summary of the characteristics of cracks that
restraint conditions, and the presence of construction and may be repaired with each procedure, the types of structures
other joints should be considered when calculating the that have been repaired, and a summary of the procedures
tensile stresses induced by concrete deformation (creep, that are used. Readers are also directed to ACI 546R,
shrinkage, temperature). Consideration should be given to 546.1R, 546.2R, RAP-1, Emmons and Emmons (1994),
cracks that develop parallel to a slab-girder joint in one-way Trout (1997), and ICRI Guideline No. 03734, which specif-
reinforced concrete slabs in which the main slab reinforcement ically address the subject of concrete repair.
is parallel to the girder as the slab spans between beams
supported by the girder. 3.2—Epoxy injection
Cracks as narrow as 0.002 in. (0.05 mm) can be bonded by
2.3—Selection of repair procedures
Based on the careful evaluation of the extent and cause of the injection of epoxy (“Crack Repair Method: Epoxy Injec-
tion” 1985). The technique generally consists of establishing
cracking, procedures can be selected to accomplish one or entry and venting ports at close intervals along the cracks,
more of the following objectives: sealing the crack on exposed surfaces, and injecting the
epoxy under pressure.
1. Restore or increase strength;
2. Restore or increase stiffness; Epoxy injection has been successfully used in the repair of
3. Improve functional performance; cracks in buildings, bridges, dams, and other types of
4. Provide watertightness; concrete structures (ACI 503R). Unless the cause of the
5. Improve appearance of the concrete surface; cracking has been corrected, however, new cracks will
6. Improve durability; and probably form near the original crack. If the cause of the
7. Prevent development of a corrosive environment at cracks cannot be removed, then three options are available:
reinforcement. 1) rout and seal the crack, thus treating it as a joint; 2) estab-
Depending on the nature of the damage, one or more lish a joint that will accommodate the movement and then
repair methods may be selected. For example, tensile inject the crack with epoxy or other suitable material; and 3)
strength may be restored across a crack by injecting it with install additional support or reinforcement at the crack location
epoxy or other high-strength bonding agent, if further to minimize movement. Epoxy materials used for structural
cracking is not anticipated (ACI 503R). It may be necessary, repairs should conform to ASTM C 881 (Type IV). ACI
however, to provide additional strength by adding reinforce- 504R describes practices for sealing joints, including joint
ment or using post-tensioning. design, available materials, and methods of application.
Cracks causing leaks in water-retaining or other storage
structures should be repaired unless the leakage is considered With the exception of certain moisture-tolerant epoxies,
minor or there is an indication that the crack is being sealed this technique is not applicable if the cracks are actively
by autogenous healing (Section 3.13). Repairs to stop leaks leaking and cannot be dried out. Wet cracks can be injected
may be complicated by a need to make the repairs while the using moisture-tolerant materials that will cure and bond in
structures are in service. the presence of moisture, but contaminants in the cracks
Cosmetic considerations may require the repair of cracks (including silt and water) can reduce the effectiveness of the
in concrete. The crack locations, however, may still be epoxy to structurally repair the cracks (Barlow 1993).
visible and, in fact, may even be more apparent due to the
repair. Depending on circumstances, some form of coating The use of a low-modulus, flexible adhesive in a crack will
over the entire surface may be required. not allow significant movement of the concrete structure
To minimize future deterioration due to the corrosion of (Gaul 1993). The effective modulus of elasticity of a flexible
reinforcement, cracks exposed to a moist or corrosive adhesive in a crack is substantially the same as that of a rigid
environment should be sealed. adhesive (Adams and Wake 1984) because of the thin layer
The key methods of crack repair available to accomplish of material and high lateral restraint imposed by the
the objectives outlined are described in Chapter 3. surrounding concrete.
CHAPTER 3—METHODS OF CRACK REPAIR Epoxy injection requires a high degree of skill for satisfactory
3.1—Introduction execution, and use of the technique may be limited by the
ambient temperature. The general procedures involved in
Following the evaluation of a cracked structure, a suitable epoxy injection are as follows (ACI 503R and RAP-1):
repair procedure can be selected. Successful repair procedures • Cleaning the cracks. The first step is to clean any
account for the cause(s) of cracking. For example, if
cracking is primarily due to drying shrinkage, then it is cracks that have been contaminated (to the extent this is
likely that, after a period of time, the cracks will stabilize. possible and practical). Contaminants, such as oil,
On the other hand, if the cracks are due to ongoing foundation grease, dirt, or fine particles of concrete, prevent epoxy
penetration and bonding, and reduce the effectiveness
of repairs. Preferably, contamination should be
removed by vacuuming or flushing with water or other
effective cleaning solutions. The solution is then
224.1R-14 ACI COMMITTEE REPORT
flushed out using compressed air and a neutralizing adhesive material begins to gel, its flow characteristics
agent or adequate time is provided for air drying. It is begin to change, and pressure injection becomes more
important, however, to recognize the practical limitations and more difficult. In the continuous mixing system,
of accomplishing complete crack cleaning. A reasonable the two liquid adhesive components pass through
evaluation should be made of the extent, and necessity, of metering and driving pumps before passing through an
cleaning. Trial cleaning may be required; automatic mixing head. The continuous mixing system
• Sealing the surfaces. Surface cracks should be sealed applies for all epoxies, including fast-setting adhesives
to keep the epoxy from leaking out before it has gelled. that have a short working life;
Where the crack face cannot be reached, but where • Injecting the epoxy. Hydraulic pumps, paint pressure
there is backfill or where a slab-on-ground is being pots, or air-actuated caulking guns may be used. The
repaired, the backfill material or subbase material is pressure used for injection should be selected carefully.
sometimes an adequate seal; however, such a condition Increased pressure often does little to accelerate the rate
can rarely be determined in advance, and uncontrolled of injection. In fact, the use of excessive pressure can
injection can cause damage such as plugging a drainage propagate the existing cracks, causing additional damage.
system. Extreme caution should be exercised when
injecting cracks that are not visible on all surfaces. A If the crack is vertical or inclined, the injection process
surface can be sealed by applying an epoxy, polyester, should begin by pumping epoxy into the entry port at the
or other appropriate sealing material to the surface of lowest elevation until the epoxy level reaches a predeter-
the crack and allowing it to harden. If a permanent mined entry port above. The lower injection port is then
glossy appearance along the crack is objectionable and capped, and the process is repeated until the crack has been
if high injection pressure is not required, a strippable completely filled and all ports have been capped.
plastic surface sealer may be applied along the face of
the crack. When the job is completed, the surface sealer For horizontal cracks, the injection should proceed
can be stripped away to expose the gloss-free surface. from one end of the crack to the other in a similar
Cementitious seals can also be used where the appear- manner. It may be required to repeat this process several
ance of the completed work is important. If extremely times until the crack is sealed. The crack is full if the
high injection pressures are needed, alternate proce- pressure can be maintained. If the pressure cannot be
dures should be followed; maintained, the epoxy is still flowing into unfilled
• Installing the entry and venting ports. Three methods portions or leaking out of the crack.
are in general use:
A low-pressure injection system is available that uses
1. Fittings inserted into drilled holes. This method discrete capsules containing a premixed epoxy. The
entails drilling a hole into the crack, approximately 3/4 in. capsules are mounted on injection ports. A spring inside
(20 mm) in diameter and 1/2 to 1 in. (13 to 25 mm) each capsule maintains a constant low pressure to dispense
below the apex of the V-grooved section, into which a a low-viscosity, long-pot-life epoxy resin into a crack.
fitting such as a pipe nipple or tire valve stem is Capillary action moves the epoxy into the cracks; and
usually bonded with an epoxy adhesive. A vacuum • Removing the surface seal. After the injected epoxy
chuck and bit, or a water-cooled core bit, is useful in has cured, the surface seal should be removed by
preventing the cracks from being plugged with grinding or other means as appropriate.
drilling dust; Another method involves the use of a vacuum or vacuum
2. Bonded flush fitting. An alternative method that is assist. There are two techniques. One technique is to entirely
frequently used to provide an entry port is to bond a enclose the cracked member with a bag, introduce the liquid
fitting flush with the concrete face over the crack. The adhesive at the bottom, and apply a vacuum at the top. The
flush fitting has an opening at the top for the adhesive other technique is to inject the cracks from one side and pull
to enter and a flange at the bottom that is bonded to the a vacuum from the other. Typically, epoxies are used;
concrete; and however, acrylics and polyesters have proven successful.
3. Interruption in seal. Another system of providing Stratton and McCollum (1974) describe the use of epoxy
entry is to omit the seal from a portion of the crack. injection as an effective intermediate-term repair procedure
This method can be used when special gasket devices for delaminated bridge decks. Epoxy resins and injection
are available that cover the unsealed portion of the procedures should be carefully selected when attempting to
crack and allow injection of the adhesive directly into inject delaminations. Unless there is sufficient depth or
the crack without leaking. anchorage to surrounding concrete, the injection process can
• Mixing the epoxy. Mixing is done by batch or continuous be unsuccessful or increase the extent of delamination.
methods. In batch mixing, the adhesive components are Smith (1992) provides information on bridge decks observed
premixed according to the manufacturer’s instructions, for up to 7 years after injection. Smithson and Whiting
usually with the use of a mechanical stirrer, like a paint- (1992) describe epoxy injection as a method to rebond
mixing paddle. Care should be taken to mix only the delaminated bridge deck overlays.
amount of adhesive that can be used before
commencement of gelling of the material. When the 3.3—Routing and sealing
Routing and sealing of cracks can be used in conditions
requiring repair where structural repair is not necessary. This
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-15
Fig. 3.2—Effect of bond breaker.
Fig. 3.1—Repair of crack by routing and sealing (Johnson Fig. 3.3—Repair using near-surface-mounted reinforcing:
1965). (1) sawcut 1/8 to 1/4 in. (3 to 6 mm) larger than bar diameter;
and (2) deformed bar or FRP bar bedded in epoxy resin.
method involves enlarging the crack along its exposed face
and filling and sealing it with a suitable joint sealant. Figure 3.1 treatment. A typical procedure for overbanding is to prepare
shows the procedure for repairing a crack. This is a common an area approximately 1 to 3 in. (25 to 75 mm) on each side
technique for crack treatment and is relatively simple of the crack by sandblasting or other means of surface
compared with the procedures and the training required for preparation, and applying a coating (such as urethane) 0.04
epoxy injection. The procedure is most applicable to approxi- to 0.08 in. (1 to 2 mm) thick in a band over the crack. Before
mately flat horizontal surfaces such as floors and pavements. overbanding in nontraffic areas, a bond breaker is sometimes
Routing and sealing can be accomplished on vertical surfaces used over a crack that has not been routed or over a crack
(with a nonsag sealant) as well as on curved surfaces (pipes, previously routed and sealed. In traffic areas, a bond breaker
piles, and poles). is not recommended. Cracks subject to minimal movement
may be overbanded, but if significant movement can take
Routing and sealing is used to treat both narrow and wide place, routing and sealing should be used in conjunction with
cracks. A common and effective use is for waterproofing by overbanding to ensure a waterproof repair.
sealing cracks on the concrete surface where water stands or
where hydrostatic pressure is applied. This treatment reduces 3.4—Near-surface reinforcing and pinning
the ability of moisture to reach the reinforcing steel or pass Near-surface reinforcing (NSR) is a method used to add
through the concrete, causing surface stains or other problems.
tensile reinforcement perpendicular to the plane of the crack.
The sealants may be any of several materials, including As shown in Fig. 3.3, a slot is sawcut across the crack, and the
epoxies, urethanes, silicones, polysulfides, asphaltic materials, slot is then cleaned. Typically, an epoxy resin is placed in the
or polymer mortars. Cement grouts should be avoided due to slot to act as a bonding agent and protective barrier to the bar
the likelihood of cracking. that is subsequently placed. Both deformed steel reinforcing
bars and precured fiber-reinforced polymer (FRP) bars are
For floors, the sealant should be sufficiently rigid to placed in the slot that is cut to approximately 0.125 in. (3 mm)
support the anticipated traffic. Load transfer at the floor wider and deeper than the diameter of the reinforcement to be
crack should be provided by aggregate interlock or dowels; installed. The reinforcing needs to be designed to increase the
otherwise, traffic loads moving across the crack may cause capacity beyond the tensile forces at the crack location.
rigid sealants to debond.
Routing and sealing consists of preparing a vertical walled 3.5.1 Conventional reinforcement—Cracked reinforced
groove at the surface typically ranging in depth from 1/4 to
1 in. (6 to 25 mm). A concrete saw or right-angle grinder concrete bridge girders have been successfully repaired by
may be used. The groove is then cleaned by airblasting, inserting reinforcing bars and bonding them in place with
sandblasting, or waterblasting, and dried. A sealant is placed epoxy (Stratton et al. 1978; Stratton 1980; “Crack Repair
into the dry groove (Fig. 3.1) and allowed to cure. Method: Conventional Reinforcement” 1985). This technique
consists of sealing the crack, drilling holes that intersect the
A variation of this procedure is to provide load transfer by
having epoxy fill or partially fill the crack by gravity. The
vertical-walled groove is used as a reservoir for epoxy that is
selected for an appropriate viscosity. The final step is to fill the
vertical-walled groove with a high-viscosity, rigid epoxy.
Active cracks should be repaired using a bond breaker at
the base of the routed channel (Fig. 3.2). A flexible sealant is
then placed in the routed channel. It is important that the
width-to-depth ratio of the channel is usually 2 or more. This
permits the sealant to respond to movement of the crack with
In some cases, overbanding (strip coating) is used inde-
pendently of or in conjunction with routing and sealing. This
method is used to enhance protection from edge spalling and,
for aesthetic reasons, to create a more uniform-appearing
224.1R-16 ACI COMMITTEE REPORT
Fig. 3.4—Reinforcing bar orientation used to affect the Fig. 3.6—Repair of crack by drilling and plugging.
repair (Stratton et al. 1978).
needed so that the problem will not merely migrate to
Fig. 3.5—Examples of external prestressing (Johnson 1965). another part of the structure. The effects of the tensioning
force (including eccentricity) on the stress within the structure
crack plane at approximately 90 degrees (Fig. 3.4), filling the should be carefully analyzed. For indeterminate structures
hole and crack with injected epoxy, and placing a reinforcing post-tensioned using this procedure, the effects of secondary
bar into the drilled hole. Typically, No. 4 or 5 (No. 13 or 16) moments and induced reactions should be considered
bars are used, extending at least 18 in. (0.5 m) each side of (Nilson 1987; Lin and Burns 1981).
the crack. The reinforcing bars can be spaced to suit the
needs of the repair. They can be placed in any desired 3.6—Drilling and plugging
pattern, depending on the design criteria and the location of Drilling and plugging a crack consists of drilling down the
the in-place reinforcement. The epoxy bonds the bar to the
walls of the hole, fills the crack plane, bonds the cracked length of the crack and grouting it to form a key (Fig. 3.6).
concrete surfaces back together in one monolithic form, and This technique is only applicable when cracks run in
thus reinforces the section. The epoxy used to rebond the
crack should have a low viscosity and conform to ASTM C reasonably straight lines and are accessible at one end. This
881 Type IV. method is most often used to repair vertical cracks in retaining
walls (“Selection of a Crack Repair Method” 1985).
3.5.2 Prestressing steel—Post-tensioning is often the
desirable solution when a major portion of a member must be A hole (typically 2 to 3 in. [50 to 75 mm] in diameter)
strengthened or when the cracks that have formed must be should be drilled, centered on and following the crack. The
closed (Fig. 3.5). This technique uses prestressing strands or hole should be large enough to intersect the crack along its
bars to apply a compressive force. Adequate anchorage full length and provide enough repair material to structurally
should be provided for the prestressing steel, and care is take the loads exerted on the key. The drilled hole should
then be cleaned, made tight, and filled with grout. The grout
key prevents transverse movements of the sections of
concrete adjacent to the crack. The key will also reduce
heavy leakage through the crack and loss of soil from behind
a leaking wall.
If watertightness is essential and structural load transfer is
not, the drilled hole should be filled with a resilient material
of low modulus instead of grout. If the keying effect is essential,
the resilient material can be placed in a second hole, with the
first being grouted.
Low-viscosity monomers and resins can be used to seal
cracks with surface widths of 0.001 to 0.08 in. (0.03 to 2 mm)
by gravity filling (Rodler et al. 1989; ACI RAP-2). High-
molecular-weight methacrylates, urethanes, and some low-
viscosity epoxies have been used successfully. The lower the
viscosity, the finer the cracks that can be filled.
The typical procedure is to clean the surface by airblasting,
waterblasting, or both. Wet surfaces should be permitted to
dry for several days to obtain the best crack filling. The
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-17
monomer or resin can be poured onto the surface and spread 3.9—Drypacking
with brooms, rollers, or squeegees. The material should be Drypacking is the hand placement of a low water content
worked back and forth over the cracks to obtain maximum
filling because the monomer or resin recedes slowly into the mortar followed by tamping or ramming of the mortar into
cracks. The use of this method on elevated slabs will require place, producing intimate contact between the mortar and the
sealing of the cracks on the bottom of the slab to contain existing concrete (U.S. Bureau of Reclamation 1975; “Crack
material from leaking through the crack. Excess material Repair Method: Drypacking” 1985). Because of the low w/cm
should be broomed off the surface to prevent slick, shining of the material, there is little shrinkage, and the patch
areas after curing. If surface friction is important, sand remains tight and can have good quality with respect to
should be broadcast over the surface before the monomer or durability, strength, and watertightness.
Drypack can be used for filling narrow slots cut for the
If the cracks contain significant amounts of silt, moisture, repair of dormant cracks. The use of drypack is not advisable
or other contaminants, the sealant cannot fill them. Water- for filling or repairing active cracks.
blasting followed by a drying time may be effective in
cleaning and preparing these cracks. Cores may be taken to Before a crack is repaired by drypacking, the portion adjacent
verify crack filling and the depth of penetration measured. to the surface should be widened to a slot about 1 in. (25 mm)
Caution should be employed to avoid cutting existing wide and 1 in. (25 mm) deep. The slot should be undercut so
reinforcement during the coring process. Cores can be tested that the base width is slightly greater than the surface width.
to give an indication of the effectiveness of the repair
method. The accuracy of the results may be limited, After the slot is thoroughly cleaned and dried, a bond coat,
however, as a function of the crack orientation or due to the consisting of cement slurry or equal quantities of cement and
presence of reinforcing steel in the core. For some polymers, fine sand mixed with water to a fluid paste consistency, or an
the failure crack will occur outside the repaired crack. appropriate latex bonding compound (ASTM C 1059),
should be applied. Placing of the drypack mortar should
3.8—Grouting begin immediately. The mortar consists of one part cement,
3.8.1 Portland-cement grouting—Wide cracks, particularly one to three parts sand passing a No. 16 (1.18 mm) sieve, and
just enough water so that the mortar will stick together when
in gravity dams (Warner 2004) and thick concrete walls, may molded into a ball by hand.
be repaired by filling with portland-cement grout. This
method is effective in stopping water leaks, but it will not If the patch must match the color of the surrounding
structurally bond cracked sections. The procedure consists of concrete, a blend of gray portland cement and white portland
cleaning the concrete along the crack; installing built-up cement may be used. Normally, about 1/3 white cement is
seats (grout nipples) at intervals astride the crack (to provide adequate, but the precise proportions can be determined only
a pressure-tight connection with the injection apparatus); by trial.
sealing the crack between the seats with a cement paint,
sealant, or grout; flushing the crack to clean it and test the To minimize shrinkage in place, the mortar should stand
seal; and then grouting the whole area. Grout mixtures may for 1/2 hour after mixing, and then be remixed before use.
contain cement and water or cement plus sand and water, The mortar should be placed in layers about 3/8 in. (10 mm)
depending on the width of the crack. The w/cm, however, thick. Each layer should be thoroughly compacted over the
should be kept as low as practical to maximize the strength surface using a blunt stick or hammer and each underlying
and minimize shrinkage. Water reducers or other admixtures layer scratched to facilitate bonding with the next layer.
may be used to improve the properties of the grout. For small There need be no time delays between layers.
volumes, a manual injection gun may be used; for larger
volumes, a pump may be used. After the crack is filled, the The repair should be cured by using either water or a curing
pressure should be maintained for several minutes to ensure compound. The simplest method of moist curing is to support a
good penetration. strip of folded wet burlap along the length of the crack.
3.8.2 Chemical grouting—Chemical grouts, such as 3.10—Crack arrest
urethanes and acrylomides, are activated by catalysts or During construction of massive concrete structures, cracks
water to form a gel, a solid precipitate, or foam that will fill
void space within concrete. The materials are primarily used due to surface cooling or other causes may develop and
for sealing cracks from water penetration. Bond strengths are propagate into new concrete as construction progresses.
typically low, so structural repairs are not made with chemical Such cracks may be arrested by blocking the crack and
grouts. Cracks in concrete as narrow as 0.002 in. (0.05 mm) spreading the tensile stress over a larger area (U.S. Army
have been filled with chemical grout. Corps of Engineers 1945).
The advantages of chemical grouts include applicability in A piece of bond-breaking membrane or a grid of steel mat
moist environments (excess moisture available), wide limits may be placed over the crack as concreting continues. A
of control of gel time, and their ability to be applied in very semicircular pipe placed over the crack may also be used
fine fractures. Disadvantages are the high degree of skill (Fig. 3.7). A description of installation procedures for semi-
needed for satisfactory use, and lack of strength. circular pipes used during the construction of a massive
concrete structure follows:
1. The semicircular pipe is made by splitting an 8 in.
(200 mm), 16 gauge pipe and bending it to a semicircular
section with an approximately 3 in. (75 mm) flange on
224.1R-18 ACI COMMITTEE REPORT
polymer concrete repair. A more detailed discussion of
polymer impregnation is given in ACI 548.1R.
3.12—Overlay and surface treatments
Cracks in structural slabs and pavements may be covered
by using either a bonded or unbonded overlay or surface
treatment. These methods do not repair cracks, but rather
hide or obscure the cracks, unless a sufficiently reinforced
overlay is installed that can handle the design loads and not
allow reflective cracking.
Fig. 3.7—Crack arrest method of crack repair. 3.13—Autogenous healing
A natural process of crack repair known as autogenous
2. The area in the vicinity of the crack is cleaned;
3. The pipe is placed in sections so as to remain centered healing can occur in concrete in the presence of moisture and
on the crack; the absence of tensile stress (Lauer and Slate 1956). It has
4. The sections are then welded together; practical application for closing dormant cracks in a moist
5. Holes are cut in the top of the pipe to receive grout environment, such as in mass concrete structures.
6. After setting the grout pipes, the installation is covered Healing occurs by formation of calcium carbonate within
with concrete placed concentrically over the pipe by hand. cracks. Calcium carbonate forms by exposure of calcium
The installed grout pipes are used for grouting the crack at a hydroxide, which is a by-product of cement hydration, to
later date. carbon dioxide in air and water (Edvardsen 1999). The
calcium carbonate that slowly precipitates is a hard, strong
3.11—Polymer impregnation material. It not only fills void space within cracks, but also
This method is used to repair cracks by impregnation with a bonds crack surfaces and restores strength to the concrete.
very low-viscosity monomer that is then polymerized in place. Healing will not occur if the crack is subjected to movement
A monomer system is a liquid consisting of monomers that during the healing period. Healing will also not occur if there
will polymerize into a solid. Suitable monomers have varying is a positive flow of water through the crack.
degrees of volatility, toxicity, and flammability, and they do
not mix with water. They are very low in viscosity, and will Saturation of the crack and the adjacent concrete with
soak into dry concrete and fill the cracks. The most common water during the healing process is essential for developing
monomer used for this purpose is methyl methacrylate. any substantial strength. Submergence of the cracked section
is desirable. Alternatively, water may be ponded on the
Monomer systems used for impregnation contain a catalyst concrete surface so that the crack is saturated. The saturation
or initiator plus the basic monomer (or combination of should be continuous for the entire period of healing. A
monomers). They may also contain a cross-linking agent. single cycle of drying and reimmersion will produce a
When heated, the monomers join together, or polymerize, drastic reduction in the amount of healing strength. Proce-
creating a tough, strong, durable plastic that greatly enhances dures to facilitate healing should begin as soon as possible
a number of concrete properties. after the crack appears. Delayed healing results in less resto-
ration of strength than does immediate correction.
If a cracked concrete surface is dried, flooded with the
monomer, and polymerized in place, some of the cracks will CHAPTER 4—REFERENCES
be filled and structurally repaired. If the cracks contain 4.1—Referenced standards and reports
moisture, however, the monomer will not soak into the
concrete at each crack face; consequently, the repair will be The standards and reports listed below were the latest
unsatisfactory. If a volatile monomer evaporates before editions at the time this document was prepared. Because
polymerization, it will be ineffective. Polymer impregnation these documents are revised frequently, the reader is advised
has not been used successfully to repair fine cracks. Polymer to contact the proper sponsoring group if it is desired to refer
impregnation has primarily been used to provide more to the latest version.
durable, impermeable surfaces (Webster et al. 1978; Hallin
1978; “Crack Repair Method: Polymer Impregnation” 1985). American Association of State Highway and Transportation
Badly fractured beams have been repaired using polymer Standard Specification for Highway Bridges
impregnation. The procedure consists of drying the fracture,
temporarily encasing it in a watertight (monomer-proof) American Concrete Institute
band of sheet metal, soaking the fractures with monomer, 201.1R Guide for Making a Condition Survey of Concrete
and polymerizing the monomer. Large voids or broken areas
in compression zones can be filled with fine and coarse in Service
aggregate before being flooded with monomer, providing a 201.2R Guide to Durable Concrete
201.3R Guide for Making a Condition Survey of Concrete
207.1R Guide to Mass Concrete
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-19
207.2R Effect of Restraint, Volume Change, and Reinforce- The above publications may be obtained from the
ment on Cracking of Mass Concrete following organizations:
207.3R Practices for Evaluation of Concrete in Existing American Association of State Highway and Transportation
Massive Structures for Service Conditions Officials
444 N Capitol Street NW
207.4R Cooling and Insulating Systems for Mass Concrete Suite 224
222R Protection in Metals in Concrete Against Corrosion Washington, D.C. 20001
224R Control of Cracking in Concrete Structures
224.2R Cracking of Concrete Members in Direct Tension American Concrete Institute
224.3R Joints in Concrete Construction P.O. Box 9094
228.2R Nondestructive Test Methods for Evaluation of Farmington Hills, MI 48333-9094
Concrete in Structures ASTM International
302.1R Guide for Concrete Floor and Slab Construction 100 Barr Harbor Drive
304R Guide for Measuring, Mixing, Transporting, and West Conshohocken, PA 19428-2959
Placing Concrete International Concrete Repair Institute
305R Hot Weather Concreting 3166 S. River Road, Suite 132
308R Guide to Curing Concrete Des Plaines, IL 60018
309R Guide for Consolidation of Concrete
309.2R Identification and Control of Visual Effects of 4.2—Cited references
Abdun-Nur, E. A., 1983, “Cracking of Concrete—Who
Consolidation Formed Concrete Surfaces
318 Building Code Requirements for Structural Concrete Cares?” Concrete International, V. 5, No. 7, July, pp. 27-30.
343R Analysis and Design of Reinforced Concrete Abeles, P. W.; Brown, E. L., II; and Morrow, J. W., 1968,
Bridge Structures “Development and Distribution of Cracks in Rectangular
345R Guide for Concrete Highway Bridge Deck Prestressed Beams During Static and Fatigue Loading,”
Journal, Prestressed Concrete Institute, V. 13, No. 5, Oct.,
Construction pp. 36-51.
345.1R Guide for Maintenance of Concrete Bridge Members
347 Guide to Formwork for Concrete Adams, R. D., and Wake, W. C., 1984, Structural Adhesive
446.1R Fracture Mechanics of Concrete: Concepts, Joints in Engineering, Elsevier Applied Science Publishers,
Ltd., Essex, England, pp. 121-125.
Models, and Determination of Material Properties
503R Use of Epoxy Compounds with Concrete Ai, H., 2000, “Investigation of the Dimensional Stability
504R Guide to Sealing Joints in Concrete Structures in DSP Cement Paste,” PhD thesis, University of Illinois at
517.2R Accelerated Curing of Concrete at Atmospheric Urbana-Champaign, 217 pp.
Pressure Alexander, A. M., 1980, “Development of Procedures for
546R Concrete Repair Guide Nondestructive Testing of Concrete Structures: Report 2,
546.1R Guide for Repair of Concrete Bridge Superstructures Feasibility of Sonic Pulse-Echo Technique,” Miscellaneous
546.2R Guide to Underwater Repair of Concrete Paper No. C-77-11, U.S. Army Engineer Waterways Exper-
548.1R Guide for the Use of Polymers in Concrete iment Station, Vicksburg, Miss., 25 pp.
RAP-1 Structural Crack Repair by Epoxy Injection, http://
Barlow, P. B., 1993, “Epoxy Injection of Cracked Slabs,”
www.concrete.org/general/RAP-1.pdf Concrete Construction, Apr., 4 pp., ftp://imgs.ebuild.com/
RAP-2 Crack Repair by Gravity Feed by Resin, http:// woc/C930253.pdf
www.concrete.org/general/RAP-2.pdf Beeby, A. W., 1983, “Cracking, Cover, and Corrosion of
Reinforcement,” Concrete International, V. 5, No. 2, Feb.,
ASTM International pp. 35-40.
C 150 Specification for Portland Cement
C 595 Specification for Blended Hydraulic Cements Bennett, E. W., and Dave, N. J., 1969, “Test Performances
C 597 Test Method for Pulse Velocity through Concrete and Design of Beams with Limited Prestress,” The Struc-
C 856 Practice for Petrographic Examination of Hardened tural Engineer (London), V. 47, No. 12, Dec., pp. 487-496.
Concrete Bentur, A.; Diamond, S.; and Berke, N. S., 1997, Steel
C 876 Test Method for Half-Cell Potentials of Uncoated Corrosion in Concrete, E&FN Spon, London, 201 pp.
Reinforcing Steel in Concrete Broms, B. B., 1965, “Crack Width and Spacing in Reinforced
C 881 Specification for Epoxy-Resin-Base Bonding Concrete Members,” ACI JOURNAL , Proceedings V. 62,
No. 10, Oct., pp. 1237-1256.
Systems for Concrete
C 1059 Specification for Latex Agents for Bonding Fresh Broms, B. B., and Lutz, L. A., 1965, “Effects of Arrange-
ment of Reinforcement on Crack Width and Spacing of
to Hardened Concrete Reinforced Concrete Members,” ACI JOURNAL, Proceedings
C 1157 Performance Specification for Hydraulic Cement V. 62, No. 11, Nov., pp. 1395-1410.
International Concrete Repair Institute
ICRI Guideline No. 03734, “Guide for Verifying Field
Performance of Epoxy Injection of Concrete Cracks”
224.1R-20 ACI COMMITTEE REPORT
Bungey, J. H., 1990, Testing of Concrete in Structures, Gaul, R. W., 1993, “Flexible Polymers and Foams for
2nd Edition, Chapman and Hall, New York, 88 pp. Crack Repair,” Concrete Repair Bulletin, June, pp. 10-12.
Butt, Y. M.; Kolbasov, V. M.; and Timashev, V. V., 1969, Gergely, P., 1981, “Role of Cover and Bar Spacing in
“High Temperature Curing of Concrete Under Atmospheric Reinforced Concrete,” Significant Developments in Engi-
Pressure,” Proceedings, 5th International Symposium on the neering Practice and Research, SP-72, American Concrete
Chemistry of Cement (Tokyo, 1968), Cement Association of Institute, Farmington Hills, Mich., pp. 133-147.
Japan, pp. 437-476.
Gergely, P., and Lutz, L. A., 1968, “Maximum Crack
Callan, E. J., 1952, “Thermal Expansion of Aggregates Width in Reinforced Concrete Members,” Causes, Mecha-
and Concrete Durability,” ACI JOURNAL, Proceedings V. 48, nism, and Control of Cracking in Concrete, SP-20, Amer-
No. 6, Feb., pp. 485-504. ican Concrete Institute, Farmington Hills, Mich., pp. 87-117.
Carlson, R. W., 1938, “Drying Shrinkage of Concrete as Haynes, H. H., 2001, “Early-Age Thermal Cracking in
Affected by Many Factors,” Proceedings, ASTM, V. 38, Lased-Screeded Concrete Slabs,” Design and Construction
Part 2, pp. 419-437. Practices to Mitigate Cracking, SP-204, E. G. Nawy, F. G.
Barth, and R. J. Frosch, eds., American Concrete Institute,
Carlson, R. W.; Houghton, D. L.; and Polivka, M., 1979, Farmington Hills, Mich., pp. 43-56.
“Causes and Control of Cracking in Unreinforced Mass
Concrete,” ACI JOURNAL, Proceedings V. 76, No. 7, July, Higginson, E. C., 1961, “Effect of Steam Curing on the
pp. 821-837. Important Properties of Concrete,” ACI JOURNAL,
Proceedings V. 58, No. 3, Sept., pp. 281-298.
Clear, K. C., and Chollar, B. H., 1978, “Styrene-Butadiene
Latex Modifiers for Bridge Deck Overlay Concrete,” Report Hallin, J. P., 1978, “Field Evaluation of Polymer Impreg-
No. FHWA-RD-78-35, Federal Highway Administration, nation of New Bridge Deck Surfaces,” Polymers in
Washington, D.C., 124 pp. Concrete, SP-58, American Concrete Institute, Farmington
Hills, Mich., pp. 267-280.
Concrete Institute of Australia, 1972, “Third Progress
Report of the Low Pressure Steam-Curing of Concrete,” Hoffman, P. C.; McClure, R. M.; and West, H. H., 1983,
North Sydney, 26 pp. “Temperature Study of an Experimental Segmental Concrete
Bridge,” Journal, Prestressed Concrete Institute, V. 28,
“Crack Repair Method: Conventional Reinforcement,” No. 2, Mar.-Apr., pp. 78-97.
1985, REMR Technical Note CS-MR-3.6, REMR Note-
book, U.S. Army Engineer Waterways Experiment Station, Holmberg, A., 1973, “Crack Width Prediction and Minimum
Vicksburg, Miss. Reinforcement for Crack Control,” Dansk Slesab for Bygn-
ingsstatitik (Copenhagen), V. 44, No. 2, June, pp. 41-50.
“Crack Repair Method: Drypacking,” 1985, REMR Tech-
nical Note CS-MR-3.8, REMR Notebook, U.S. Army Engi- Houghton, D. L., 1972, “Concrete Strain Capacity Tests—
neer Waterways Experiment Station, Vicksburg, Miss. Their Economic Implications,” Economical Construction of
Concrete Dams, American Society of Civil Engineers, New
“Crack Repair Method: Epoxy Injection,” 1985, REMR York, pp. 75-99.
Technical Note CS-MR-3.9, REMR Notebook, U.S. Army
Engineer Waterways Experiment Station, Vicksburg, Miss. Houghton, D. L., 1976, “Determining Tensile Strain
Capacity of Mass Concrete,” ACI JOURNAL, Proceedings
“Crack Repair Method: Polymer Impregnation,” 1985, V. 73, No. 12, Dec., pp. 691-700.
REMR Technical Note CS-MR-3.11, REMR Notebook,
U.S. Army Engineer Waterways Experiment Station, Vicks- Houk, I. E.; Borge, O. E.; and Houghton, D. L., 1969,
burg, Miss. “Studies of Autogenous Volume Change in Concrete in
Dworshak Dam,” ACI JOURNAL, Proceedings V. 66, No. 7,
Dakhil, F. H.; Cady, P. D.; and Carrier, R. E., 1975, July, pp. 560-568.
“Cracking of Fresh Concrete as Related to Reinforcement,”
ACI JOURNAL, Proceedings V. 72, No. 8, Aug., pp. 421-428. Illston, J. M., and Stevens, R. F., 1972, “Long-Term Cracking
in Reinforced Concrete Beams,” Proceedings, Institution of
Darwin, D.; Browning, J.; and Lindquist, W. D., 2004, Civil Engineers (London), Part 2, V. 53, pp. 445-459.
“Control of Cracking in Bridge Decks: Observations from
the Field,” Cement, Concrete and Aggregates, ASTM Inter- Jastrzebski, Z. D., 1961, Nature and Properties of Engi-
national, V. 26, No. 2, Dec., pp. 148-154. neering Materials, John Wiley and Sons, New York, 571 pp.
Davis, H. E., 1940, “Autogenous Volume Change of Johnson, S. M., 1965, Deterioration, Maintenance, and
Concrete,” Proceedings, ASTM, V. 40, pp. 1103-1110. Repair of Structures, McGraw-Hill Book Co., New York,
Dusinberre, D. M., 1945, “Numerical Methods for
Transient Heat Flow,” Transactions, American Society of Kaminetzky, D., 1981, “Failures During and After
Mechanical Engineers, V. 67, Nov., pp. 703-712. Construction,” Concrete Construction, V. 26, No. 8, Aug.,
Edvardsen, C., 1999, “Water Permeability and Autogenous
Healing of Cracks in Concrete,” ACI Materials Journal, Kelly, J. W., 1981, “Cracks in Concrete: Part 1, Part 2,”
V. 96, No. 4, July-Aug., pp. 448-454. Concrete Construction, V. 26, No. 9, Sept., pp. 725-734.
Emmons, P. H., and Emmons, B. W., 1994, Concrete Repair Kirkbride, T. W., 1971a, “Review of Accelerated Curing
and Maintenance Illustrated, R. S. Means Co., 300 pp. Procedures,” Precast Concrete (London), V. 1, No. 2, Feb.,
Frosch, R. J., 1999, “Another Look at Cracking and Crack
Control in Reinforced Concrete,” ACI Structural Journal, Kirkbride, T. W., 1971b, “Burner Curing,” Precast
V. 96, No. 3, May-June, pp. 437-442. Concrete (London), V. 1, No. 11, Nov., pp. 644-646.
CAUSES, EVALUATION, AND REPAIR OF CRACKS 224.1R-21
Knab, L. I.; Blessing, G. V.; and Clifton, J. R., 1983, Rodler, D. J.; Whitney, D. P.; Fowler, D. W.; and Wheat,
“Laboratory Evaluation of Ultrasonics for Crack Detection D. L., 1989, “Repair of Cracked Concrete with High Molec-
in Concrete,” ACI JOURNAL, Proceedings V. 80, No. 1, Jan.- ular Weight Methacrylates,” Polymers in Concrete:
Feb., pp. 17-27. Advances and Applications, SP-116, American Concrete
Institute, Farmington Hills, Mich., pp. 113-127.
Lauer, K. R., and Slate, F. O., 1956, “Autogenous Healing
of Cement Paste,” ACI JOURNAL, Proceedings V. 53, No. 10, Sansalone. M., 1997, “Impact-Echo: The Complete
June, pp. 1083-1098. Story,” ACI Structural Journal, V. 94, No. 6, Nov.-Dec.,
Libby, J. R., 1977, Modern Prestressed Concrete, 2nd
Edition, Van Nostrand Reinhold, New York, pp. 388-390. Sansalone, M., and Carino, N. J., 1988, “Laboratory and
Field Studies of the Impact-Echo Method for Flaw Detection
Lin, T. Y., and Burns, N. H., 1981, Design of Prestressed of Concrete,” Nondestructive Testing of Concrete, SP-112,
Concrete Structures, 3rd Edition, John Wiley & Sons, New American Concrete Institute, Farmington Hills, Mich., pp. 1-20.
York, 646 pp.
Sansalone, M., and Carino, N. J., 1989, “Detecting Delam-
Malhotra, V. M., and Carino, N. J., eds., 2004, Handbook inations in Concrete Slabs with and without Overlays Using
on Nondestructive Testing of Concrete, 2nd Edition, CRC the Impact-Echo Method,” ACI Materials Journal, V. 86,
Press, Boca Raton, Fla., 384 pp. No. 2, Mar-Apr., pp. 175-184.
Mansfield, G. A., 1948, “Curing—A Problem in Thermo- Schmitt, T. R., and Darwin D., 1999, “Effect of Material
dynamics,” Rock Products, V. 51, No. 8, Aug., p. 212. Properties on Cracking in Bridge Decks,” Journal of Bridge
Engineering, ASCE, V. 4, No. 1, Feb., pp. 8-13.
Mast, R. F., 1981, “Roof Collapse at Antioch High
School,” Journal, Prestressed Concrete Institute, V. 26, No. 3, “Selection of a Crack Repair Method,” 1985, REMR
May-June, pp. 29-53. Technical Note CS-MR-3.1, REMR Notebook, U.S. Army
Engineer Waterways Experiment Station, Vicksburg, Miss.
Mattock, A. H., and Chan, T. C., 1979, “Design and
Behavior of Dapped-End Beams,” Journal, Prestressed Shideler, J. J., and Toennies, H. T., 1963, “Plant Drying
Concrete Institute, V. 24, No. 6, Nov.-Dec., pp. 28-45. and Carbonation of Concrete Block-NCMA-PCA Coopera-
tive Program,” ACI JOURNAL, Proceedings V. 60, No. 5,
Mindess, S.; Young, J. F.; and Darwin, D., 2003, May 1963, pp. 617-634. Also, Development Department
Concrete, 2nd Edition, Prentice-Hall, Upper Saddle River, Bulletin No. D64, Portland Cement Association, Skokie, Ill.
N.J., 644 pp.
Smith, B. J., 1992, “Epoxy Injection of Bridge Deck
Nilson, A. H., 1987, Design of Prestressed Concrete, 2nd Delaminations,” Transportation Research Record 1533,
Edition, John Wiley and Sons, New York, 526 pp. Transportation Research Board, National Research Council,
Nurse, R. W., 1949, “Steam Curing of Concrete,” Magazine
of Concrete Research (London), V. 1, No. 2, June, pp. 79-88. Smithson, L. D., and Whiting, J. E., 1992, “Rebonding
Delaminated Bridge Deck Overlays,” Concrete Repair
PCI Committee on Quality Control Performance Criteria, Digest, V. 3, No. 3, June-July, pp. 100-101.
1983, “Fabrication and Shipment Cracks in Prestressed
Hollow-Core Slabs and Double Tees,” PCI Journal, V. 28, Snowdon, L. C., and Edwards, A. G., 1962, “The Moisture
No. 1, Jan.-Feb., pp. 18-39. Movement of Natural Aggregate and Its Effect on
Concrete,” Magazine of Concrete Research (London), V. 14,
PCI Committee on Quality Control Performance Criteria, No. 41, July, pp. 109-116.
1985, “Fabrication and Shipment Cracks in Precast or
Prestressed Beams and Columns,” PCI Journal, V. 30, No. 3, Stratton, F. W., 1980, “Custom Concrete Drill Helps
May-June, pp. 24-49. Repair Shear Cracks in Bridge Girders,” Concrete Interna-
tional, V. 2, No. 9, Sept., pp. 118-119.
PCI Energy Committee, 1981, Discussion of “Accelerated
Curing of Concrete at Atmospheric Pressure—State of the Stratton, F. W.; Alexander, R.; and Nolting, W., 1978,
Art,” ACI JOURNAL, Proceedings V. 78, No. 4, July-Aug., “Cracked Structural Concrete Repair through Epoxy Injec-
pp. 320-324. tion and Rebar Insertion,” Report No. FHWA-KS-RD.78-3,
Kansas Department of Transportation, Topeka, Kans., Nov.,
Pickett, G., 1956, “Effect of Aggregate on Shrinkage of 56 pp.
Concrete,” ACI JOURNAL, Proceedings V. 52, No. 5, Jan.,
pp. 581-590. Stratton, F. W., and McCollum, B. F., 1974, “Repair of
Hollow or Softened Areas in Bridge Decks by Rebonding
Powers, T. C., 1975, “Freezing Effects in Concrete,” with Injected Epoxy Resin or Other Polymers,” Report No. K-
Durability of Concrete, SP-47, American Concrete Institute, F-72-5, State Highway Commission of Kansas, July, 104 pp.
Farmington Hills, Mich., pp. 1-11.
Suprenant, B. A., and Malisch, W. R., 1999, “The Fiber
Price, W. H., 1982, “Control of Cracking During Construc- Factor,” Concrete Construction, Oct., 4 pp., ftp://
tion,” Concrete International, V. 4, No. 1, Jan., pp. 40-43. imgs.ebuild.com/woc/C99J043.pdf
Priestley, M. J., N., 1978, “Design of Concrete Bridges for Transportation Research Board, 1979, “Durability of
Temperature Gradients,” ACI JOURNAL, Proceedings V. 75, Concrete Bridge Decks,” NCHRP Synthesis of Highway
No. 5, May, pp. 209-217. Practice No. 57, Transportation Research Board, Wash-
ington, D.C., May, 61 pp.
Rehm, G., and Eligehausen, R., 1977, “Lapped Splices of
Deformed Bars Under Repeated Loadings (Ubergreifungs-
tosse von Rippenstahlen unter nicht ruhender Belastung),”
Beton und Stahlbeton (Berlin), No. 7, pp. 170-174.
American Concrete Institute®
Advancing concrete knowledge
As ACI begins its second century of advancing concrete knowledge, its original chartered purpose
remains “to provide a comradeship in finding the best ways to do concrete work of all kinds and in
spreading knowledge.” In keeping with this purpose, ACI supports the following activities:
· Technical committees that produce consensus reports, guides, specifications, and codes.
· Spring and fall conventions to facilitate the work of its committees.
· Educational seminars that disseminate reliable information on concrete.
· Certification programs for personnel employed within the concrete industry.
· Student programs such as scholarships, internships, and competitions.
· Sponsoring and co-sponsoring international conferences and symposia.
· Formal coordination with several international concrete related societies.
· Periodicals: the ACI Structural Journal and the ACI Materials Journal, and Concrete International.
Benefits of membership include a subscription to Concrete International and to an ACI Journal. ACI
members receive discounts of up to 40% on all ACI products and services, including documents, seminars
and convention registration fees.
As a member of ACI, you join thousands of practitioners and professionals worldwide who share a
commitment to maintain the highest industry standards for concrete technology, construction, and
practices. In addition, ACI chapters provide opportunities for interaction of professionals and practitioners
at a local level.
American Concrete Institute
38800 Country Club Drive
Farmington Hills, MI 48331
Causes, Evaluation, and Repair of Cracks
in Concrete Structures
The AMERICAN CONCRETE INSTITUTE
was founded in 1904 as a nonprofit membership organization dedicated to public
service and representing the user interest in the field of concrete. ACI gathers and
distributes information on the improvement of design, construction and
maintenance of concrete products and structures. The work of ACI is conducted by
individual ACI members and through volunteer committees composed of both
members and non-members.
The committees, as well as ACI as a whole, operate under a consensus format,
which assures all participants the right to have their views considered. Committee
activities include the development of building codes and specifications; analysis of
research and development results; presentation of construction and repair
techniques; and education.
Individuals interested in the activities of ACI are encouraged to become a member.
There are no educational or employment requirements. ACI’s membership is
composed of engineers, architects, scientists, contractors, educators, and
representatives from a variety of companies and organizations.
Members are encouraged to participate in committee activities that relate to their
specific areas of interest. For more information, contact ACI.